UNRAVELING PHOTONIC BANDS:
CHARACTERIZATION OF SELFCOLLIMATION EFFECTS IN TWO
DIMENSIONAL PHOTONIC CRYSTALS
A Dissertation
Presented to
The Academic Faculty
By
Tsuyoshi Yamashita
In Partial Fulfillment
Of the Requirements for the Degree
Doctor of Philosophy in
Materials Science and Engineering
Georgia Institute of Technology
August, 2005
Copyright © Yamashita 2005
UNRAVELING PHOTONIC BANDS:
CHARACTERIZATION OF SELFCOLLIMATION EFFECTS IN TWO
DIMENSIONAL PHOTONIC CRYSTALS
Approved by:
Dr. Christopher Summers, Chairman
School of Materials Science and
Engineering
Georgia Institute of Technology
Dr. James Meindl
Microelectronics Research Center
Georgia Institute of Technology
Dr. Mo Li
School of Materials Science and
Engineering
Georgia Institute of Technology
Dr. GeeKung Chang
School of Electrical and Computer
Engineering
Georgia Institute of Technology
Dr. Brent Carter
School of Materials Science and
Engineering
Georgia Institute of Technology
Dr. Zhong Lin Wang
School of Materials Science and
Engineering
Georgia Institute of Technology
Date Approved: June 14, 2005
It is my task to convince you not to turn away because you don't understand it. You see
my physics students don't understand it... That is because I don't understand it. Nobody
does.
Richard P. Feynman, QED, The Strange Theory of Light and Matter
This thesis is dedicated to my wife, Zhuqing, who has faithfully and steadfastly supported
me throughout the entirety of my pursuit of this degree. Without a doubt, this thesis
would not have been possible without her diligent and constant care.
iv
ACKNOWLEDGEMENT
The author would like to acknowledge his advisor, Dr. Christopher Summers, and
the members of the committee, Dr. James Meindl, Dr. GeeKung Chang, Dr. Brent Carter,
and Dr. Mo Li, for their invaluable support and input.
The author also thanks the National Science Foundation for the graduate research
fellowship and the United States Army Research Office’s Multi University Research
Initiative contract DAAA 190110603 for providing the funding which made the work
in this thesis possible.
Special thanks go out to Dr. Won Park and his student Ethan Schronbrun at the
University of Colorado, and Dr. Jeff King and Dr. Elton Graugnard at Georgia Tech for
providing the support and facilities necessary to perform measurement on the fabricated
structures. Special acknowledgements also go to Curtis Neff and Wenjie Mai for their
assistance in the 3D simulation and atomic force microscopy measurements, respectively.
The author would like to acknowledge the support of the Microelectronics
Research Center (MiRC) cleanroom staff for their hard work and dedication for
maintaining and servicing the equipment in the cleanroom which has allowed the
research in this thesis possible. Special acknowledgement goes out to Vinh Nguyen and
Devin Brown.
The author would also like to acknowledge Dr. Susumu Noda and the member’s
of his research group in the Kyoto University in Japan for hosting an exchange program
during the second summer of my research. The experience and knowledge gained as well
v
as the discussions following the visit have been a continual source of motivation for the
current work.
To conclude, the author would like to acknowledge the members of the faculty,
staff, and students at Georgia Tech who have provided him support and valuable
discussions on the work contained within this thesis.
vi
TABLE OF CONTENTS
ACKNOWLEDGEMENT.................................................................................................iv
LIST OF TABLES.............................................................................................................ix
LIST OF FIGURES............................................................................................................x
SUMMARY ..................................................................................................................xvi
CHAPTER 1: INTRODUCTION TO PHOTONIC CRYSTALS.....................................1
CHAPTER 2: MODELING AND SIMULATION OF PHOTONIC CRYSTAL
PROPERTIES...........................................................................................11
Introduction...................................................................................................................11
Analysis Methods..........................................................................................................12
Simulation Techniques..................................................................................................17
Plane Wave Expansion Method................................................................................17
Finite Difference Time Domain Simulation.............................................................21
Photonic Crystal Effective Index Model.......................................................................30
SelfCollimation in the Square Lattice Photonic Crystal..............................................42
Robustness of the SelfCollimation Effect...................................................................44
Application of SelfCollimated Beams.........................................................................51
Optical Interconnects................................................................................................52
FabryPerot Interferometer.......................................................................................56
Discussion.....................................................................................................................60
CHAPTER 3: FABRICATION OF 2D PHOTONIC CRYSTALS................................62
Introduction...................................................................................................................62
Substrate: Silicon on Insulator (SoI).............................................................................63
Amorphous Silicon on Insulator (ASoI)...................................................................64
vii
Single Crystal SoI.....................................................................................................70
Patterning: Electron Beam Lithography (EBL)............................................................71
Principle of Operation...............................................................................................72
Optimization.............................................................................................................77
Patterns Generated....................................................................................................84
Pattern Transfer: Plasma Etching..................................................................................85
Principle of Operation...............................................................................................86
NonChlorine Based Etch Results............................................................................93
ICP Etch Optimization..............................................................................................94
Device Etching........................................................................................................116
PostEtch Processing...............................................................................................118
Discussion...................................................................................................................122
CHAPTER 4: MEASUREMENT OF 2D PHOTONIC CRYSTAL PROPERTIES....124
Introduction.................................................................................................................124
Band Structure Measurements....................................................................................124
Principle of Operation.............................................................................................125
Results.....................................................................................................................129
SelfCollimation Measurements.................................................................................133
Design.....................................................................................................................133
Measurement Setup.................................................................................................135
Results.....................................................................................................................136
Discussion...................................................................................................................141
CHAPTER 5: CONCLUSION.......................................................................................144
APPENDIX A .................................................................................................................148
viii
MFile: initTM2.m......................................................................................................148
MFile: solveTM2.m...................................................................................................150
APPENDIX B .................................................................................................................151
Mfile script: PREP_A.m............................................................................................151
Mexfile: a2de.c..........................................................................................................155
TE Mode FDTD Library.............................................................................................161
APPENDIX C: TRAVELER FOR THE FABRICATION PROCESS..........................162
REFERENCES...............................................................................................................167
ix
LIST OF TABLES
Table 1. Table of DealGrove model constants for oxidation of silicon.........................66
Table 2. Overview of etches performed for optimization of etch rates, selectivity, and
sidewall profile................................................................................................115
x
LIST OF FIGURES
Figure 1. Schematics of the drilling directions to form Yablonovite
4143
.........................4
Figure 2. a.) 2D
51
and b.) 3D
48
photonic crystals fabricated using lithography and
microelectronics technology.............................................................................5
Figure 3. Simulation of line defect waveguides showing a.) sharp bend
12
, b.) beam
splitting
15
, c.) leakage free intersections
14
, and d.) coupling between
branches
13
..........................................................................................................6
Figure 4. a.) Schematic of a drop filter composed of photonic crystals with slightly
varying sizes utilized to filter out selected wavelength channels from the line
defect waveguide b.) SEM picture of the cavity c.) SEM picture of waveguide
region d.) Drop channel intensity
23
...................................................................7
Figure 5. Simulations of negative index phenomena such as focusing and imaging in
a.)
39
and b.) and negative refraction in c.)
38
......................................................8
Figure 6. Experimental observation of negative refraction
27
...........................................8
Figure 7. Simulation results showing a.) beam bending
34
and b.) beam splitting with
selfcollimated beams
33
.....................................................................................9
Figure 8. Experimental demonstration of selfcollimated beams
34
..................................9
Figure 9. Schematic of a square lattice photonic crystal made of high dielectric constant
pillars...............................................................................................................13
Figure 10. The allowed wave vector surface for the TM mode of a square lattice photonic
crystal..............................................................................................................13
Figure 11. The band diagram for the TM mode of a square lattice photonic crystal
.........................................................................................................................14
Figure 12. a.) Allowed wave vector contours for the first band of a square lattice
photonic crystal b.) Methodology for using the allowed vector contour to
calculate the refraction angle at an interface...................................................16
Figure 13. Dielectric function calculated for 529 Fourier coefficients (23x23) with two
different methods. a.) Averaging the dielectric function to a coarse grid b.)
Utilizing the center section of the Fourier transform of a fine grid................20
Figure 14. Band diagram calculated using the FDTD method (dots) compared with those
using the PWE method for the Γ−Χ direction................................................26
xi
Figure 15. Band diagram showing the light line for the air and substrate radiation modes
.........................................................................................................................32
Figure 16. Models for fitting the allowed wave vector curve for the ΓM direction.......33
Figure 17. Effective index values calculated for the square lattice photonic crystal.......40
Figure 18. Beam width correlation between the model and FDTD simulation...............41
Figure 19. Phase correlation between the model and the FDTD simulation....................41
Figure 20. The normalized frequency of the selfcollimation point and the slope of the
curvature for a square lattice photonic crystal made of high index pillars.....42
Figure 21. The normalized frequency of the selfcollimation point and the slope of the
curvature for a square lattice photonic crystal made of low index holes........44
Figure 22. Schematic of the photonic crystal slab investigated
36
.....................................45
Figure 23. The band diagram and the allowed wave vector curves for the photonic crystal
slab
36
...............................................................................................................46
Figure 24. Propagation of a Gaussian beam in a.) silica and b.) photonic crystal slab
36
.47
Figure 25. Beam spreading in a photonic crystal compared to isotropic media
36
............48
Figure 26. Beam spreading as a function of the wavelength for systematic errors
36
.......49
Figure 27. Beam spreading as a function of error magnitude for a.) random distribution
and b.) normal distribution of pillar sizes
36
....................................................51
Figure 28. Band diagram showing the band gap for r = 0.2 and r = 0.3 in the silicon/silica
structure
36
........................................................................................................53
Figure 29. A plot of the intensity of a 90° reflection of a selfcollimated beam by a band
gap photonic crystal simulated by FDTD
36
....................................................54
Figure 30. Beam spread and transmission coefficient for a Gaussian beam traveling
through 85.6 µm and one 90° turn
36
...............................................................54
Figure 31. Noninteracting crossing of selfcollimated beams
36
......................................55
Figure 32. Routing three parallel beams with different wavelengths and widths within a
single signal layer using the photonic crystal virtual waveguide
36
.................56
Figure 33. Transmission properties for photonic crystal FPI with a.) plane wave
incidence and b.) an 8.5 µm wide Gaussian beam..........................................58
xii
Figure 34. Simulations of the interferometer with photonic crystal mirrors with a.) free
space and b.) selfcollimating photonic crystal in between the mirrors.........59
Figure 35. Flow chart of fabrication processes................................................................63
Figure 36. Schematic of a PECVD system.......................................................................65
Figure 37. 3D images of AFM scans for silicon oxide. a.) Deposited by PECVD and b.)
Grown using wet oxidation.............................................................................67
Figure 38. Cracking of amorphous silicon films grown on thermally oxidized wafers.
The depositions were performed at: a.) 150°C for 30 min. b.) 300°C for 30
min and left at room temperature for 1 week. c.) 150°C for 45 min. d.) 300°C
for 30 min and removed from the platen immediately...................................69
Figure 39. 3D images of AFM scans for amorphous silicon deposited over a.) PECVD
oxide and b.) wet oxidation grown oxide........................................................70
Figure 40. Amorphous silicon deposited at 150°C for 30min and etched in a buffered
oxide etch for 10min showing that it can form a free standing film...............70
Figure 41. Schematic of the major components of a.) the JEOL JBX9300FS EBL system
and b.) the sample holder cassette.beam.........................................................73
Figure 42. Spin speed vs. thickness of the resulting resist thickness for ZEP520A
electron beam resist.........................................................................................78
Figure 43. Increase in the diameter of circles written in the EBL system with respect to
the dose and the location within the pattern....................................................80
Figure 44. Example of stitching error caused by improper calibration of the height of the
sample.............................................................................................................82
Figure 45. EBL writing time normalized to 1 mm
2
exposure area for various test patterns
.........................................................................................................................83
Figure 46. Optical image of the device pattern written ZEP520A resist on an ASoI.....85
Figure 47. Basic configuration of an ICP plasma etching machine.................................87
Figure 48. Schematic showing the profile control provided by a sidewall passivation etch
where polymerizing species coat the sidewalls..............................................90
Figure 49. Cross section of a chlorine etch with microtrenching effect...........................92
Figure 50. Angled view and a cross section of grass formation in a chlorine/oxygen
plasma etch......................................................................................................92
xiii
Figure 51. Cross section of 2 µm trenches etched using an SF6, O2, and Ar etch in the
RIE..................................................................................................................93
Figure 52. 1 µm sized pillars etched in silicon utilizing the Bosch process....................94
Figure 53. Monitored DC bias for two cleaning processes on the Plasmatherm ICP......96
Figure 54. Pure chlorine etch of silicon trenches with a pitch of a.) 2 µm and b.) 600 nm
.........................................................................................................................98
Figure 55. Cross sections of silicon etched utilizing a mixture of Cl
2
and CF
4
. The
concentration of CF
4
in the recipe and the pitch of the trenches are labeled.
.......................................................................................................................100
Figure 56. Cross section of silicon etched utilizing a mixture of Cl
2
and CHF
3
. The
concentration of CHF
3
in the recipe and the pitch of the trenches are labeled.
.......................................................................................................................102
Figure 57. Cross section of silicon etched utilizing a mixture of Cl
2
and BCl
3
. The
concentration of BCl
3
in the recipe and the pitch of the trenches are labeled
.......................................................................................................................103
Figure 58. Cross section of silicon etched utilizing a mixture of Cl
2
and C
4
F
6
. The
concentration of C
4
F
6
in the recipe and the pitch of the trenches are labeled
.......................................................................................................................105
Figure 59. Etch rate and selectivity with respect to the RF
1
power...............................106
Figure 60. Etch rate and selectivity with respect to RF
2
power.....................................108
Figure 61. Silicon etch rate for different process pressures and RF
2
power with respect to
total gas flow.................................................................................................110
Figure 62. Resist etch rate for different process pressures and RF
2
power with respect to
total gas flow.................................................................................................110
Figure 63. Selectivity of silicon versus ZEP520A resist for different process pressures
and RF
2
power with respect to total gas flow...............................................111
Figure 64. Polymerization on the side walls of deep etching recipes. a.) 4min recipe b.)
10min recipe..................................................................................................112
Figure 65. Deep etching characteristics of silicon showing increasing microtrenching
with decreasing C
4
F
6
concentration..............................................................114
Figure 66. Deep vertical trenches etched by Cl
2
/C
4
F
6
plasma by ramping both the
concentration of C
4
F
6
and the RF
1
power from 10% to 20% concentration and
3W to 7.5W, respectively..............................................................................114
xiv
Figure 67. Test etch for verification of recipe consistency for ASoI device fabrication117
Figure 68. Compilation of SEM pictures of devices etched in ASoI and SoI wafers. a.)
Low magnification overall view. b.) Magnified end of input waveguide. c.)
Input interface of photonic crystal on ASoI. d.) Input end of photonic crystal
on SoI with modified design.........................................................................117
Figure 69. 45° angled view of the edge of a cleaved ASoI sample on two locations of the
same sample..................................................................................................119
Figure 70. 30° angled view of holes etched in an SoI showing the rough surface of the
bottom oxide.................................................................................................120
Figure 71. Circular patterns plasma etched into silicon with a.) 3 min. soak in BOE b.)
20min soak in BOE.......................................................................................121
Figure 72. Tearing and deformation of photonic crystals that were completely undercut
by BOE etching.............................................................................................121
Figure 73. AFM scan of a smoothed ASoI wafer...........................................................122
Figure 74. Measurement setup for the reflectivity measurements.................................126
Figure 75. Reference scan for the reflectivity setup showing the effects of OH bond
absorption in the fiber and the detector sensitivity drop off.........................127
Figure 76. Two graphical illustrations for coupling of out of plane incident radiation into
the photonic crystal for analysis of reflectivity data. a.) wave vector analysis
b.) band diagram analysis.............................................................................128
Figure 77. Reflectivity measurements on a.) a thin film region and b.) the photonic
crystal region of an ASoI substrate with respect to the incident angle.........130
Figure 78. Band diagrams a.) obtained from the reflectivity measurements and b.)
compared with simulation for the second band............................................131
Figure 79. Overlay of the band diagram from the measurement and simulation utilizing
values corrected for the thickness and the native oxide................................132
Figure 80. A schematic of the device design for observation of selfcollimation..........134
Figure 81. A schematic of the measurement setup for top view imaging of the photonic
crystal device................................................................................................136
Figure 82. Top view IR images of the various regions of the photonic crystal device..138
Figure 83. Output region imaged for the single crystal SoI showing selfcollimation
effect for the TE mode with an empty reference and a TM mode incident for
comparison....................................................................................................139
xv
Figure 84. Output region imaged for the single crystal SoI with 424.3 nm lattice
parameter showing the band gap and large divergence for wavelengths close
to the band gap..............................................................................................139
Figure 85. Band diagram of the first band for the TE and TM mode showing the
frequency range measured showing the selfcollimation effect...................140
Figure 86. Output region imaged for the ASoI showing selfcollimation effect for the TE
mode with the reference and a schematic for comparison............................142
Figure 87. Band diagram for the ASoI sample showing selfcollimation effect............142
xvi
SUMMARY
Photonic crystals, periodic dielectric structures that control photons in a similar
way that atomic crystals control electrons, present opportunities for the unprecedented
control of light. Photonic crystals display a wide gamut of properties, such as the
photonic band gap, negative index of refraction, slow or stationary modes, and
anomalous refraction and propagation effects. This thesis investigates the modeling,
simulation, fabrication, and measurement of twodimensional square lattice photonic
crystals. An effective index model was developed to describe the propagation of
electromagnetic waves in the media and applied to characterize the behavior of self
collimated beams to discern the effect of the photonic crystal on the evolution of the
amplitude and phase of the propagating beam. Potential applications include optical
interconnects and stand alone devices such as filters and lasers. Based on design
parameters from the simulations, two dimensional photonic crystals were fabricated on
amorphous and single crystal silicononinsulator substrates utilizing electron beam
lithography and inductively coupled plasma etching. A unique etching process utilizing a
combination of Cl
2
and C
4
F
6
gases was developed and characterized which displayed a
vertical profile with a sidewall angle of under 1 degree from vertical and very smooth
sidewalls for features as small as 150 nm. The high quality of the etching was the key to
obtaining extremely low loss, low noise structures, making feasible the fabrication of
large area photonic crystal devices that are necessary to measure propagation phenomena.
Reflectivity measurements were used to directly observe the photonic band structure with
excellent correlation with theory. A device was designed and fabricated which
successfully verified the prediction of the simulations through measurements of the self
xvii
collimation effect across a broad range of infrared wavelengths. A solid foundation for
the necessary components (simulation, modeling, design, fabrication, and measurement)
of twodimensional photonic crystal has been demonstrated. Elements from solid state
physics, materials science, optics, and electromagnetics were incorporated to further the
understanding of the mechanism of beam propagation in photonic crystals and illuminate
the vast potential of research in periodic media.
1
CHAPTER 1
INTRODUCTION TO PHOTONIC CRYSTALS
Ever since the discovery of atoms and crystals, periodic structures have been an
integral part of the understanding of material systems. Recently, research in engineered
periodic structures in the same size range as the wavelength of interest has flourished.
Electromagnetic waves have garnered the most intense attention beginning with the
proposal by Yablonovitch
2
and John
3
on the inhibition of spontaneous emission and the
confinement of photons by structures exhibiting a photonic band gap. In addition to
electromagnetic crystals, acoustic signals
4
and even water waves
5
have been
demonstrated to display band gap properties in structures with a periodic elastic modulus.
Artificially engineered periodic structures allow control over every detail, even the unit
cell. This intriguing field continues to develop new breakthroughs as creativity and
innovation forge crystals with unique and novel properties.
This thesis delves into the properties of twodimensional photonic crystals, one of
the simplest classes of structures available within this topic. Even though it is such a
simple structure, the methods of analyzing and interpreting the properties are still being
developed. The methods of modeling and simulating the properties of periodic structures
were introduced and developed for the behavior of electrons in atomic crystals, where the
Schrödinger’s Equation reigns supreme
6,7
:
(
)
0)(
2
2
2
=Ψ−+Ψ∇ rVE
m
h
Equation 1
2
where Ψ is the electron wave function, m the mass, ħ the Planck’s constant divided by 2π,
E the energy, and V(r) the electric potential as a function of position r. Maxwell’s
Equations serve as the counterpart in describing photons, or electromagnetic waves. The
Maxwell’s Equations can be rearranged to parallel the exact same format as the
Schrödinger’s Equations
8
:
0
2
0
2
=+∇ EkE
0
2
0
2
=+∇ BkB
Equation 2
where
2
2
0
2
)(
⎟
⎠
⎞
⎜
⎝
⎛
=
λ
π
εrk
where E is now the electric field, B the magnetic field, and k
0
the wave vector in free
space, ε(r) the dielectric constant as a function of position r, and λ the wavelength of light.
This parallelism led naturally to the band structure formalism to describe the properties of
photonic crystals. The initial development of photonic crystals mirrored the phenomena
already characterized for atomic crystals, such as the band gap and defect modes from
doping
911
. Once the band gap effect was established, development in the field was
driven towards the approaches taken by the microwave and radio frequency (RF) fields
where photonic band gap materials were substituted for the perfect electrical conductor in
frequency ranges, such as the visible and infrared (IR), where metallic conductors
exhibited significant loss. Size issues challenged the community until fabrication
techniques matured in the mid 1990’s allowing fabrication of structures in the submicron
range. This approach gave birth to line defect waveguides
1219
and high Qfactor
cavities
1921
which burgeoned beyond the limitations of its longer frequency range
3
counterparts to demonstrate devices such as add/drop filters
22,23
for dense wavelength
division multiplexing (DWDM) applications.
Recently, the study of bulk propagation effects, such as superprisms
2429
(large
refraction angles with small deviation in input angle), selfcollimation
2936
(reduction of
the spreading of a beam as it propagates), and negative index of refraction
3739
, has
attracted large attention. These phenomena display parallels to the electronic band
structure, but take advantage of the unique properties of photons. The electronic band
structure is governed by the solution of the periodic form of Schrödinger’s Equation
7
,
coupled with the knowledge of the properties of electrons, such as Pauli Exclusion
Principle and Hund’s Rule. When characterizing the electronic properties of a crystal,
the emphasis is on the density of states and the FermiDirac distribution. By filling the
band structure from the lowest energy and considering the behavior of the highest energy
electrons, the properties of insulators, conductors, and semiconductors can be
obtained
6,7,40
. In addition, due to the tractability of the electron by electric and magnetic
fields and the polycrystalline nature of most materials, the direction, or wave vector, of
the electrons in a crystal is often overlooked. On an atomic level, the electron will travel
only in the propagation direction allowed by the crystal, but by changing its direction, it
will macroscopically follow the direction imposed by the potential difference set by a
voltage gradient. Photons are fundamentally different from electrons in that they do not
follow the Pauli Exclusion Principle. As bosons, photons obey the BoseEinstein
distribution which allows an infinite number of photons to occupy the same state
6,40
. The
density of states is no longer a focus in the analysis. Instead, the wave vector and the
directionality of the band structure become the primary focus of the interpretation. The
4
wave vector of a photon is difficult to modify without material boundaries, thus discrete
propagation directions and phenomena which take advantage of controlling the wave
vector of a photon, such as refraction, become possible. Photonic crystals utilize the
periodic arrangement of dielectric materials to control the wave vector of photons. The
selfcollimation effect investigated in this thesis is a phenomenon which utilizes this
distinct property of a photon to control the propagation of a beam of light inside the
photonic crystal.
Various methods exist for the fabrication of periodic structures. For large
structures, with feature sizes on the order of cm or greater, bulk machining techniques are
adequate. The first demonstration of a photonic band gap was in the Yablonovite
4143
structure, a 3cylinder diamond cubiclike lattice structure, in the microwave wavelength,
which allowed construction utilizing mechanical drilling of a dielectric slab. This
structure, schematically shown in Figure 1, was fabricated and successfully demonstrated
a photonic band gap for the 10~13GHz wavelengths
42
. Even though the photonic band
filler
Figure 1. Schematics of the drilling directions to form Yablonovite
4143
.
5
gap was demonstrated at microwave wavelengths, interest in band gap structures failed to
develop due to the availability of metals to act as perfect reflectors. However, the race to
fabricate photonic crystal structures that display a complete band gap in the visible and
near infrared wavelengths was started and arguably still continues today
4449
. Three
classes of fabrication methods emerged for creating photonic crystals. Lithographic
techniques developed in the microelectronic industry provide an ideal method for the
fabrication of twodimensional photonic crystals. Threedimensional logpile structures
have been fabricated utilizing lithography by stacking alternate layers through wafer
bonding
49,50
and through sequential layer growth and planarization using chemical
mechanical polishing
47,48
. An example of a twodimensional line defect waveguide
51
and
a logpile structure
48
are shown in Figure 2. Selfassembly of monodispersed colloidal
particles proved to be a breakthrough in providing an affordable method for fabricating
the opal and inverse opal structures which, with an appropriate index of refraction,
exhibit complete photonic band gaps. Holography techniques utilizing the interference
of multiple beams to create periodic structures give the ability to fabricate defect free
filler
Figure 2. a.) 2D
51
and b.) 3D
48
photonic crystals fabricated using lithography and microelectronics
technology
b.)
a.)
6
large area photonic crystals with any degree of periodicity by combining different
numbers of beams. In this thesis, fabrication of twodimensional photonic crystals
utilizing electron beam lithography coupled with thin film deposition and plasma etching
was investigated.
With the successful demonstration of the photonic band gap, focus turned to the
engineering of devices utilizing the photonic band structure. Numerous theoretical
studies were conducted on twodimensional structures as the computational capability
could accommodate the size of the simulation. Functionalities in band gap guided line
defect waveguides produced many of the initial simulated functionalities
1215
, as shown in
Figure 3. The silicononinsulator (SoI) structure consisting of a high index (n = 3.45)
filler
Figure 3. Simulation of line defect waveguides showing a.) sharp bend
12
, b.) beam splitting
15
, c.)
leakage free intersections
14
, and d.) coupling between branches
13
a.)
b.)
d.)
c.)
7
silicon layer on top of silicon oxide layer (n = 1.45) provided the index confinement in
the offplane direction allowing for a structure closely resembling an ideal two
dimensional structure. Photonic crystals fabricated on SoI have successfully
demonstrated the theoretical calculations of defect waveguides
51
with sharp bends and
resonant cavity devices. A schematic of a drop filter composed of a line defect
waveguide and resonant cavities, along with an SEM image and the measured frequency
response are shown in Figure 4
23
.
Negative index phenomena, such as imaging, focusing, and negative refraction
have also been simulated
3739
and experimentally observed
27
, as shown in Figure 5 and
Figure 6. The concept of bulk propagation through the photonic crystal having self
collimation and lenslike effects was first proposed by Kosaka
30
qualitatively utilizing the
curvature of the equifrequency contour. Figure 7 reveals further simulation results and
theoretical developments for the propagation of selfcollimated beams demonstrating the
ability to make sharp turns and split beams as was demonstrated for the line defect
waveguide
33,34
. These effects were demonstrated by Prather
34,35
, as seen in Figure 8,
filler
Figure 4. a.) Schematic of a drop filter composed of photonic crystals with slightly varying sizes
utilized to filter out selected wavelength channels from the line defect waveguide b.) SEM picture of
the cavity c.) SEM picture of waveguide region d.) Drop channel intensity
23
8
Figure 5. Simulations of negative index phenomena such as focusing and imaging in a.)
39
and b.) and
negative refraction in c.)
38
Figure 6. Experimental observation of negative refraction
27
a.)
c.)
b.)
9
Figure 7. Simulation results showing a.) beam bending
34
and b.) beam splitting with selfcollimated
beams
33
filler
Figure 8. Experimental demonstration of selfcollimated beams
34
a.)
b.)
10
utilizing structures fabricated on a SoI with electron beam lithography. Twodimensional
photonic crystal devices have proven to be a fruitful area of research fulfilling the
promises and expectations of the modeling and simulation results.
This study focuses on further understanding light propagation through a two
dimensional photonic crystal. The thesis is divided into three main chapters focusing on
modeling and simulation, fabrication, and property measurement of twodimensional
photonic crystals. Chapter 2 details the simulation methodology utilized for calculating
the photonic band structure and modeling the devices. An effective index model for the
propagation of Gaussian beams in a photonic crystal was developed, followed by
simulations of applications utilizing selfcollimated beams. Chapter 3 provides an
extensive overview of the fabrication process with an emphasis on the development of a
unique plasma etch that produced highly anisotropic and very smooth sidewalls necessary
for photonic crystal devices. An overview of the measurement techniques and the results
for the fabricated devices are given in Chapter 4. Each chapter ends with a discussion to
highlight the key points presented. Finally, Chapter 5 concludes the thesis with an
overview of the accomplishments, their significance, and outlook for the work presented.
11
CHAPTER 2
MODELING AND SIMULATION OF PHOTONIC CRYSTAL
PROPERTIES
Introduction
Simulation has been a cornerstone of the photonic crystal community ever since
its inception when the existence of the photonic band gap was postulated through the
results of theoretical simulations
2,3
. Indeed, the photonic crystal community has reversed
the centuries old method of modeling and simulation being created to explain an
observed phenomenon. Photonic crystal research has benefited from the advances in the
microelectronic industry, not just in fabrication techniques, but in the computing power
that it has provided to make accurate simulations. Photonic crystal research is an area
which exemplifies the revolution in the scientific community, where the models and the
simulation methods have reached an accuracy which gives confidence that the
phenomena observed in the simulation can be experimentally verified. This chapter
introduces two methods for analyzing the properties of photonic crystals, the band
diagram and the allowed wave vector surface. After introducing these methods, detailed
overviews of the plane wave expansion and finite difference time domain methods, the
two most common simulation methods for the analysis of photonic crystal, are given.
The majority of the simulations performed for this thesis was developed and ran in the
Matlab environment and a section is devoted within the description of each method to
address issues encountered in the code development. The next section describes the
development of an effective index of refraction model to describe propagation of a
12
Gaussian beam through a photonic crystal. A survey to determine the selfcollimation
frequencies in a square lattice photonic crystal was conducted followed by an analysis of
the robustness of the selfcollimation phenomenon to manufacturing errors. Finally,
simulation results for several applications of selfcollimated beams in photonic crystals
are presented.
Analysis Methods
Simulations of photonic crystal properties begin with the calculation of the band
structure. The band structure is calculated by utilizing the Bloch boundary condition,
which is the periodic boundary condition with a specified wave vector to add a phase
change at the boundary. Simulations can calculate or identify the frequencies of the
mode which is stable with the imposed Bloch condition. By calculating these modes for
the wave vectors in the first Brillouin zone, the band structure of the photonic crystal can
be found. The band structure for the wave vectors outside of the first Brillouin zone are
then found by folding the band diagram along the directions of periodicity
6,52
. The wave
vector space, analogous to reciprocal lattice space, is a mapping of the direction and
period of a wave into a point. The vector defined by the origin and a point in the wave
vector space corresponds to a wave which has the wave fronts propagating along the
wave vector direction and the period proportional to the inverse of the vector length.
When compared to the reciprocal lattice, the crystal plane mapped in reciprocal lattice
corresponds to the equiphase plane of a plane wave depicted by the same wave vector.
Several graphical representations similar to solid state physics have become
common in displaying the band properties of the photonic crystals. The band structure
for the transverse magnetic (TM) slab mode of a square lattice photonic crystal made of
13
dielectric (n = 3.3) pillars with a radius of 20% of the lattice constant, shown in Figure 9,
will be used as an example for this section. It is worth noting that the TMslab mode
corresponds to the TE photonic crystal mode as the slab mode calculation is based on the
cross section while the topdown view is the reference plane for the photonic crystal
calculation. For this thesis, the slab mode conventions are utilized when referring to the
modes. The allowed wave vector surface, depicted in Figure 10, displays a three
dimensional plot of the solutions solved for each wave vector. Only the points in the
filler
Figure 9. Schematic of a square lattice photonic crystal made of high dielectric constant pillars
Figure 10. The allowed wave vector surface for the TM mode of a square lattice photonic crystal
14
irreducible Brillouin zone, the triangle which can be repeated to reproduce the entire band
diagram, are plotted. Even though this representation is compact and shows a complete
representation of the band structure, it is visually too complex and no valuable
information can be garnered from it. A representation including only one band can be
utilized to show the curvature of the surface but will not be used in this thesis
34
.
The band diagram is the most common representation of the band structure of
photonic crystals. This representation plots the boundary of the irreducible Brillouin
zone, the smallest area of the wave vector space that, through symmetry operations, can
form the whole wave vector space. Figure 11 shows an example of the band diagram.
The xaxis is divided into regions representing the line segments connecting the
Γ−Χ−Μ−Γ points in wave vector space. The band diagram allows identification of the
location and width of the band gap and the movement of bands with respect to changing
conditions. The band diagram is often expressed in normalized frequency and wave
filler
Figure 11. The band diagram for the TM mode of a square lattice photonic crystal
Γ
Χ
Μ
15
vector due to the scalability of Maxwell’s Equations given that the structure is not small
enough to require consideration of quantum effects. In the normalized frequency
notation, the frequency is scaled so that a plane wave in free space at a normalized
frequency of 1 has a period equal to the lattice constant. This corresponds to:
c
a
n
π
ω
ω
2
=
Equation 3
where ω
n
is the normalized frequency, ω is the angular frequency, a is the lattice constant,
and c is the speed of light.
The representation of the band structure most useful for propagation through a
photonic crystal is the allowed wave vector contour, also called the equifrequency
contour. This representation is obtained by taking one band in the band surface and
taking slices with equal frequencies. Each curve represents the allowed wave vector
surface for that frequency and can be utilized in the same manner as in refractive optics to
obtain the propagation direction and coupling at an interface. The allowed wave vector
contours along with a schematic describing the methodology of utilizing these contours
for determining the refraction angle is given in Figure 12. The allowed wave vector for
an isotropic material is a circle, as seen on the left side of the interface. To graphically
determine the refraction angle, the wave vector of the incoming wave is graphed from the
periphery of the circle to the origin. The transverse component of the wave vector is
conserved, and a line is drawn perpendicular to the interface that intersects the allowed
wave vector curve of the second material. The wave will couple into the second material
with a wave vector equal to the vector from the origin to the intersection point
53
. This
principle applies even for the allowed wave vector curve of a photonic crystal, which can
filler
16
Figure 12. a.) Allowed wave vector contours for the first band of a square lattice photonic crystal b.)
Methodology for using the allowed vector contour to calculate the refraction angle at an interface
take on shapes that are not circular or elliptical as in isotropic materials. The allowed
wave vector surface of the first band reveals some noteworthy properties of the photonic
crystal. Near the center of the first band, the frequency is the lowest, corresponding to
waves with a lattice constant which is much larger than the periodicity of the lattice. In
this regime, the wave sees an average dielectric constant and the allowed wave vector is
circular as in an isotropic material. As the wave vector reaches a value which is near the
edge of the Brillouin zone, the shape gradually changes from a circle to a shape
resembling the lattice, or a square. Near the top of the first band, near the M point, the
allowed wave vector once again shifts towards a circle, but now with the center located
on the M point rather than on the Γ point. This trend where the allowed wave vector
curve near a symmetrical point in the wave vector space approximates a circle is the
source of the negative index and the selfcollimation effects.
Interface
n
1
n
2
(
θ
)
k
0
n
1
k
0
n
2
(
θ
Φ
Γ
Μ
Χ
First Band
b.)
a.)
k
y
k
1
k
2
S
2
k
x
17
Simulation Techniques
Since the exact solution to Maxwell’s Equation for photonic crystals cannot be
obtained, a numerical method must be employed to find approximate solutions describing
the system. Due to the rapidly improving performance of personal computers and
workstations, these numerical calculations can be performed in a reasonable time frame
for research purposes. All programs in this proposal use the Matlab programming
language running on high end personal computers with CPU powers ranging from
2.8GHz to 3.4GHz Pentium IV processors and 3GB of memory.
Two different approaches to simulate photonic crystals have been pursued in this
thesis. The first method, the plane wave expansion (PWE) method, is a straight forward
numerical approximation of the solutions to the wave equation using Fourier expansion
of the dielectric constant and the electric/magnetic field as a function of position. The
second method utilized is Finite difference time domain (FDTD) simulation. In this
method, an electromagnetic (EM) wave traveling through a grid representing the photonic
crystal is monitored to discern the interaction of the EM wave with the photonic crystal.
The FDTD simulation is a very flexible technique allowing for the simulation of
infinitely periodic structures as well as discrete devices containing defects and waveguide
structures.
Plane Wave Expansion Method
The PWE method is a numerical method for solving the decoupled Maxwell’s
Equations. For this method, the form of the decoupled equations are
54
:
{
}
)()(
)(
1
2
2
rE
c
rE
r
ω
ε
=×∇×∇
18
)()(
)(
1
2
2
rH
c
rH
r
ω
ε
=
⎪
⎭
⎪
⎬
⎫
⎪
⎩
⎪
⎨
⎧
×∇×∇
Equation 4
where E is the electric field and H the magnetic field. Then the dielectric function is
approximated by a twodimensional Fourier series expansion of the form
54
:
)exp()(
)(
1
rGiG
r
G
⋅=
∑
κ
ε
Equation 5
where κ(G) are the twodimensional Fourier coefficients of the dielectric function in
space. Furthermore, through the Bloch’s Theorem, the solution to the differential
equation can also be expressed as a Fourier series expansion
54
:
{
}
∑
⋅+=
G
nknk
rGkiGErE )(exp)()(
{
}
∑
⋅+=
G
nknk
rGkiGHrH )(exp)()(
Equation 6
where k is now the wave vector. When these equations are substituted back into
Maxwell’s Equations, a set of linear equations are formed, which can be solved using
linear algebra techniques
54
:
{ }
∑∑∑
=×+×+−−
G
nk
nk
nk
G G
GE
c
GEGkGkGG )()'()'()')('(
2
2
'
ω
κ
{ }
∑∑∑
=×+×+−−
G
nk
nk
nk
G G
GH
c
GHGkGkGG )()'()'())('(
2
2
'
ω
κ
Equation 7
The equations on the left hand side can be written as square matrices if G and G’ are of
the same size while the right hand side is a constant times a vector of E or H.
Furthermore, the same vector of E
kn
as on the right side can also be factored out of the
left hand square matrix to form the common eigenvalue problem of the form:
19
xAx
λ
=
Equation 8
where A is the square matrices formed by κ, k, G, and G’; λ is ω
kn
2
/c
2
; and x is a vector
of E
kn
or H
kn
. Therefore, the solutions λ and x can be numerically solved using linear
algebra functions available in commercial software (such as the eig/eigs function in
Matlab).
In the PWE method, input values corresponding to the physical geometry of the
photonic crystals, number of expansions to take in the Fourier expansion, and the k vector
to be evaluated results in the eigenvalue solution λ and the eigenvector solution x. For
each calculation, there are numerous nontrivial solutions λ with their corresponding
eigenvectors with each nontrivial solution corresponding to a different band in the band
diagram. The band diagram is the plot of the ω (calculated from λ) against the input k
vector. The accuracy of the PWE method is determined through the number of Fourier
expansions of the dielectric function and the electric/magnetic field. Most simulations
are conducted with between 1000 and 8000 plane waves in the expansion
55,56
. Due to
computational limitations, a larger expansion is impractical. This limit puts a severe
restriction on the accuracy of this method since the number of plane waves is given by
the formula:
(
)
( )
2
3
122____#
123____#
−=
−=
nDwavesplaneof
nDwavesplaneof
Equation 9
Where n is the number of independent Fourier coefficients along each principal axis (κ(G)
= κ
*
(G) so they are not independent). It is clearly seen that for a threedimensional case,
the dielectric function and the solution can only be expanded in at most 10 Fourier
coefficients per side. For the twodimensional case, a more reasonable expansion in 30
20
45 Fourier coefficients can be performed. Care must be taken in calculating the Fourier
coefficients. To decrease the Fourier coefficients to the requisite number, the value of the
dielectric constant can be averaged over the fine grid to fit it to a coarse grid. This
method is required for simulations which directly utilizes the dielectric function in the
calculations. However, for the PWE method, only the Fourier coefficients are used. A
more accurate depiction of the structure can be obtained by first taking the fast Fourier
transform of a very fine grid, and then decreasing the number of Fourier coefficients by
utilizing the values symmetrically around the origin. The difference can be seen in
Figure 13. Utilizing the fine grid decreases the sharp corners which occur when the
dielectric function is averaged first. Utilizing sufficient conditions, the PWE method can
be used to calculate the band structure of the photonic crystal quickly and accurately. All
of the band structures in this thesis are calculated using the PWE method unless
otherwise stated.
The Matlab implementation of the PWE method is very straight forward, as the
environment was created to handle matrix operations. The mfile functions written to
filler
Figure 13. Dielectric function calculated for 529 Fourier coefficients (23x23) with two different
methods. a.) Averaging the dielectric function to a coarse grid b.) Utilizing the center section of the
Fourier transform of a fine grid
a.)
b.)
21
calculate the band diagram for the TM mode of a twodimensional photonic crystal is
given in APPENDIX A. The program was divided into two functions to make the code
simple and efficient to use. The initTM2.m function takes the inputs of a matrix
containing the inverse of the dielectric constant, the G vectors of the unit cell (x and y
directions for square lattice), and the number of Fourier coefficients to expand along each
direction. The initTM2.m function initializes all of the variables necessary so that only
the wave vector and the number of bands to solve for needs to be input for the
solveTM2.m function. This format makes programming to solve for different dielectric
structures and different configurations of the band structure, such as the band diagram
and the allowed wave vector contours, straight forward by defining the appropriate loops
in a script. The Matlab function for solving the eigenvalues of a matrix (eigs), is a
precompiled code written in Fortran, thus the speed of the code was comparable to codes
written in C or Fortran. Code written in Fortran was still faster, but the added flexibility
and the ease of integrating high level graphical and signal processing functions within the
program made the developed code much more powerful in application. The
corresponding TE mode program requires only slight modifications and is not included in
the Appendices.
Finite Difference Time Domain Simulation
The PWE method is useful for perfectly periodic materials where a small number
of Fourier coefficients may be used to accurately depict both the dielectric modulation
and the solution. However, many geometries of interest are not perfectly periodic and are
too complex to accurately depict using a small number of Fourier coefficients. For these
cases, the finite difference time domain (FDTD) simulation method can be used. FDTD
22
has the advantage of using a grid to define the material properties so sharp discontinuities
can be accurately modeled compared to using a Fourier series. However, due to the use
of square or cubic grids, smooth curves need to be approximated using blocks causing a
“staircase” effect
57
. The evolution of an EM wave is followed through discretized time
steps in this finite grid.
The FDTD method can be derived from the Maxwell’s Equations by discretizing
the curl equations in the form (for simplicity, the assumptions of linear, isotropic,
nondispersive, noloss material is made)
57
:
E
t
H
×∇−=
∂
∂
µ
1
H
t
E
×∇=
∂
∂
ε
1
Equation 10
Expanding the curl operators yields six coupled scalar equations
57
:
⎥
⎦
⎤
⎢
⎣
⎡
∂
∂
−
∂
∂
=
∂
∂
y
E
z
E
t
H
z
y
x
µ
1
⎥
⎦
⎤
⎢
⎣
⎡
∂
∂
−
∂
∂
=
∂
∂
z
E
x
E
t
H
x
z
y
µ
1
⎥
⎦
⎤
⎢
⎣
⎡
∂
∂
−
∂
∂
=
∂
∂
x
E
y
E
t
H
y
x
z
µ
1
⎥
⎦
⎤
⎢
⎣
⎡
∂
∂
−
∂
∂
=
∂
∂
z
H
y
H
t
E
y
z
x
ε
1
⎥
⎦
⎤
⎢
⎣
⎡
∂
∂
−
∂
∂
=
∂
∂
x
H
z
H
t
E
z
x
y
ε
1
⎥
⎦
⎤
⎢
⎣
⎡
∂
∂
−
∂
∂
=
∂
∂
y
H
x
H
t
E
x
y
z
ε
1
Equation 11
23
These equations are discretized to form the update equations to step through each time
step and are the basis of the FDTD method for EM radiation. For the case where one
dimension extends to infinity with no variation, these equations can be simplified since
all of the partial derivatives with respect to z vanish
57
:
⎥
⎦
⎤
⎢
⎣
⎡
∂
∂
−=
∂
∂
y
E
t
H
z
x
µ
1
⎥
⎦
⎤
⎢
⎣
⎡
∂
∂
=
∂
∂
x
E
t
H
z
y
µ
1
⎥
⎦
⎤
⎢
⎣
⎡
∂
∂
−
∂
∂
=
∂
∂
y
H
x
H
t
E
x
y
z
ε
1
⎥
⎦
⎤
⎢
⎣
⎡
∂
∂
=
∂
∂
y
H
t
E
z
x
ε
1
⎥
⎦
⎤
⎢
⎣
⎡
∂
∂
−=
∂
∂
x
H
t
E
z
y
ε
1
⎥
⎦
⎤
⎢
⎣
⎡
∂
∂
−
∂
∂
=
∂
∂
x
E
y
E
t
H
y
x
z
µ
1
Equation 12
Notice that the first three equations depend on only H
x
, H
y
, and E
z
while the last three are
also dependent only on each other. These two cases are the TE and the TM modes
respectively. Therefore, when simulating a twodimensional structure, a smaller
simulation using only half of the variables can be conducted for the TE and TM cases
separately. A leapfrog scheme where the E and H components are displaced half a cell
width apart and also half a time step apart is used to maximize the efficiency of the
algorithm
57
.
24
The FDTD method can be used for many different types of simulations. It can
simulate both the PBG structure and the dispersion characteristics in an infinite, as well
as a finite, structure. In addition, the FDTD method has been used to simulate complex
cases such as propagation along an offaxis direction in a twodimensional structure
58
.
Band Diagram Calculation
The FDTD technique can be used to calculate the band diagram for perfectly
periodic structures in two and threedimensions as well as structures with periodicity in
two dimensions and anisotropy in the third dimension, such as waveguides. To
understand how to simulate the band structure using the FDTD method, the physical
significance of each point in the band diagram needs to be examined. As described in the
characterization section, each point on the band diagram represents an EM field pattern,
which corresponds to a stationary field comparable to a standing wave pattern in a
vibrating string. Therefore, to simulate the band diagram, a long simulation of the
periodic structure is performed to isolate the stationary signal from the background noise.
All field intensities deviating from the stationary field pattern will travel through the grid
and vanish when the time average is taken over a sufficiently long simulation. When
taking the boundary conditions, recall that the solution to the Maxwell’s Equations can be
expanded in a Fourier series as in the PWE case:
{
}
∑
⋅+=
G
nknk
rGkiGErE )(exp)()(
{
}
∑
⋅+=
G
nknk
rGkiGHrH )(exp)()(
Equation 13
25
Substituting r+L for r in these expressions where L is the principle lattice vector for the
unit cell and solving in terms of E
kn
(r) and H
kn
(r)
56
:
{
}
{
}
LkirELrGkiGELrE
nk
G
nknk
⋅=+⋅+=+
∑
exp)()()(exp)()(
{
}
{
}
LkirHLrGkiGHLrH
nk
G
nknk
⋅=+⋅+=+
∑
exp)()()(exp)()(
where
1)exp( =⋅ LGi
Equation 14
Therefore, the boundary conditions are the periodic boundary condition with an
appropriate phase shift applied proportional to the k vector. Many initial field patterns
were tested including the delta function, random number generator, and a superposition
of plane waves as described in the paper by Chan et. al.
56
. For simulations of the
primitive unit cell, all initial conditions worked well. However, for nonprimitive unit
cells, the superposition of plane waves was necessary to meet the boundary conditions.
The Fourier transform of the resulting data was analyzed for peaks corresponding to each
data point on the band diagram. Sample band diagram calculated using a 50x50 grid for
the same dielectric profile used in the PWE section was shown in Figure 14. The results
show that long time steps are necessary to accurately simulate the band diagram.
Even though perfectly periodic materials shed light on the possibilities of
photonic crystals, real applications often fall far short of the perfectly periodic conditions
used for the simulation. One main deviation is the waveguide structure where the third
dimension is confined through total internal reflection rather than extending to infinity, as
the twodimensional case assumes. In a waveguide structure, the electromagnetic energy
26
Figure 14. Band diagram calculated using the FDTD method (dots) compared with those using the
PWE method for the Γ−Χ direction
travels in both the waveguide and in the surrounding cladding area due to the evanescent
field extending from the boundary of the waveguide
53
. Also, this confinement in the third
direction can cause different modes to form in the third dimension complicating the
analysis. The FDTD method can simulate the waveguide structure for comparison with
the twodimensional case simulated using the PWE method or the FDTD method.
Results have shown that by utilizing the effective index calculated for the slab mode of
an index confined waveguide layer, an accurate simulation of the band structure can be
obtained by twodimensional calculations for the threedimensional slab structure
59
.
Device Simulation
In addition to producing the band structure, the FDTD technique can simulate the
behavior of finite structures and interfaces between photonic crystals and other materials.
Plane wave expansion
50,000 time steps
150,000 time steps
27
In this type of simulation, an EM wave travels from air or another outside medium into
the photonic crystal. The electric and magnetic fields can be recorded to monitor the
evolution of the fields with any arbitrary structure. In this manner, a theoretical
experiment can be performed to predict the behavior of actual photonic crystal devices.
Simulation of a device utilizing FDTD has the same basic steps as an actual
experiment. First, a sample is created by defining the dielectric function for the
simulation space. Then a light source is simulated as either a monochromatic sine wave
or a Gaussian or modulated Gaussian at the inputs of the device. The response of the
device is measured by recording the EM fields at the output location. The advantages of
the FDTD method over an actual experiment are not only in the ease of creating and
measuring a device, but in the degree of control it has on the data to be collected. By
utilizing a Gaussian or a modulated Gaussian source in time, a range of frequencies can
be measured in a single simulation. Also, field values can be measured in locations
which can not be probed in an actual experiment along with the measurement not
interfering with the propagating waves. The main limitation of this method is the
computational size. Due to the shear size of the data which needs to be stored for such a
simulation, computational space sizes are limited to around 50 million points. This is less
than 400 grid points along each axis for a threedimensional simulation, which limits the
ability of 3D FDTD to simulate realistic devices. However, for twodimensional
problems, 7000 grid points along each axis is possible allowing for the simulation of
structures closely resembling an actual device. The finite simulation size requires a
boundary condition which absorbs all of the radiation reaching the edge of the simulation
space. This is accomplished through the Berenger’s perfectly matched layer (PML). The
28
principle behind the PML lies in placing a lossy material at the edge of the simulation
space with no reflections back into the grid. By satisfying the following conditions, a
reflectionless interface for normal incidence can be achieved
57
:
21
ε
ε
=
=
21
µ
µ
=
=
11
Γ
εµσσ =
Equation 15
where ε and µ are the dielectric constant and magnetic permeability of the two materials,
and σ
*
and σ are the magnetic and electric conductivity of the PML material. To increase
the performance of the PML for nonnormal incidence, the two conductivities are
gradually increased following a third or fourth order polynomial to slowly absorb the
impinging radiation
57
.
Numerous types of simulations can be performed utilizing the twodimensional
FDTD method. Transmission and reflection measurements and refraction angle
measurements are commonly simulated. Selfcollimation and negative index can also be
demonstrated utilizing this method. All of the simulation figures shown in the
introduction chapter were calculated utilizing the twodimensional FDTD technique. In
this thesis, measurement of the properties of the selfcollimated beams as it propagates
inside of a photonic crystal and simulations of the applications for selfcollimated beams
are conducted using this method.
Matlab Implementation
FDTD program is composed of a large number of additions, subtractions,
multiplications, and divisions as a series of these operations must be performed at each
29
grid point. This brute force approach to calculation is not well suited for a high level
programming environment such as Matlab, and resulted in a simulation speed which was
3 orders of magnitude slower for the Matlab code compared to a code written in C or
Fortran. This difference arises from the high level variable type and variable consistency
tests that Matlab performs at each iteration. To overcome this issue, the bulk of the
calculations involving the floating point operations, were written in the C programming
language and linked to Matlab through compiling the C program as a mexfunction inside
of the Matlab environment. Through this operation, the speed of the simulation was
increased by a factor of 100. Another increase in speed, by a factor of 10, was obtained
by changing the compiler from the standard “lcc” compiler into the Microsoft Visual
Studio C++ compiler. The program was ran on a Windows XP Professional computer,
thus the C compiler by Microsoft was found to perform the best. When utilizing the C
mexfile for the FDTD code, the simulation ran with a speed that was comparable to, and
even faster than, some FDTD codes available for download.
The two main components of the code with PML boundary conditions are given
in APPENDIX B. The mfile script is similar to the initiation function for the PWE
method. It requires a matrix with the inverse of the dielectric constant and the size of
each grid point. Based on these two values, the script declares all of the other variables,
including the PML parameters. The mexfile includes the bulk of the calculations and
performs one time step. After each time step, the updated fields are returned to the
Matlab environment where the fields can be plotted in real time or a value can be
monitored and plotted onto the screen. Since the compiled mexfile utilizes the same
location in memory as the Matlab code, the overhead of returning the simulation back
30
into the Matlab environment is small. However, by having access to the simulation data
in real time, the powerful post processing capabilities of the Matlab environment can be
utilized to perform complex analysis and functions on the data without the need to write
extensive code to add into the program or to store an extremely large amount of data. A
precompiled addin for the Matlab environment with help files and example programs
was created for the two dimensional TE mode FDTD with periodic, Bloch, and absorbing
boundary conditions. This has been made available upon request as stated in the
Appendix.
Photonic Crystal Effective Index Model
Propagation through a photonic crystal is a complex phenomenon requiring a
renewed look at the current models. The index of refraction is the property used to
describe propagation of light inside of a material. Since atoms and molecules are much
smaller than the wavelength of light, the light only sees an average dielectric constant.
The frequency response for ordinary dielectrics are dependent on resonances of the
various charged entities within the material for which models have been developed to
characterize its frequency response such as the Debye model
60
. Photonic crystals obey a
different model for their frequency dependent properties. The lattice constant of the
photonic crystal is on the same order of magnitude as the wavelength of light it is
designed to operate in. Therefore, the light waves interact strongly with the geometry of
the structure resulting in features such as the band gap, selfcollimation, and negative
index of refraction. In this section, the characteristics of the photonic crystal slab are
introduced, followed by the development of an effective index model which describes the
31
propagation behavior of a Gaussian beam along the ΓM direction of a square lattice
photonic crystal.
Before embarking on the task of developing an effective index model for
propagation through a photonic crystal, an overview of the twodimensional photonic
crystal slab is given to understand the system being simulated, fabricated, and measured.
The twodimensional photonic crystal slab is a class of photonic crystals where the
periodic structure is fabricated on a thin film of high index material sandwiched between
two layers of low index material. In the case of the silicononinsulator substrate, the
high index layer is silicon (n = 3.45), the low index layer on the bottom is silicon oxide (n
= 1.45), and the top layer is either air (n = 1) or another coat of oxide. The TE and TM
slab modes for this structure can be calculated for a symmetrical case, and simulated for
the nonsymmetrical cases
61
. These modes have an effective index which describes their
propagation wave vectors. Twodimensional band structure calculations utilizing this
effective index have yielded good agreements with full threedimensional calculations
59
.
Another concern for the photonic crystal slab is the loss of the mode to the air layer and
substrate layer. The coupling of the mode to an isotropic media on the top and bottom
surface of the photonic crystal can be treated utilizing the allowed wave vector curve in a
similar way to the refraction angle analysis. If the mode inside of the photonic crystal
has a smaller wave vector than the wave vector in the free space or substrate material, the
mode can couple into a radiation mode
62
. This condition is identical to the case for total
internal reflection. A graphical representation for this condition is the light line drawn on
the band diagram, as shown in Figure 15. The light line, or light cone in two dimensions,
is the line drawn in the normalized band diagram where the magnitude of the normalized
filler
32
Figure 15. Band diagram showing the light line for the air and substrate radiation modes
frequency is the wave vector divided by the index of refraction of the media. All modes
above the light line have the possibility of coupling into a radiation mode. From the band
diagram shown, it is apparent that only the first band is entirely within the light line,
while parts of the second to fourth bands remain below the light line depending on the
index of the substrate. Staying under the light line is critical for a successful photonic
crystal device, thus this thesis focuses on the top of the first band where it is guaranteed
that the mode is always below the light line.
Figure 12 shows the shape of the allowed wave vector curves in the first band of a
square lattice photonic crystal. At low frequencies, near the Γpoint or center of the
Brillouin zone, the allowed wave vector curves are circular. This corresponds to the
physical interpretation applied earlier that the wavelength is much greater than the
periodicity resulting in an average dielectric constant felt by the wave regardless of the
33
direction of the wave propagation. As the wave vector approaches the edge of the
Brillouin zone, the shape changes. The ΓM direction exhibits an anomaly. As the
contours are followed from the Γ point to the M point, the curvature changes from
convex to concave with respect to the Γ point. At the point where the concavity changes,
the curvature of the wave vector curve is zero and a beam of light will travel without
spreading
30
. A model for the property of the portion of the curve beyond the self
collimation point was proposed as a material exhibiting a negative dielectric constant
39
:
2
1
0
0
ε
ε
ε
−
=
Equation 16
This results in an allowed wave vector curve corresponding to a hyperbola. Developing
this approach further, this thesis investigates the use of elliptical and hyperbolic fitting of
the wave vector curve. Schematics of the model fitting utilizing the wave vector contour
for a square lattice photonic crystal simulated for a silicon pillar / silicon oxide matrix
slab waveguide is given in Figure 16. Models were investigated in this thesis to fit the
wave vector contour with a circle, ellipse, and a hyperbola by adjusting the index of
filler
Figure 16. Models for fitting the allowed wave vector curve for the ΓM direction
34
refraction. The circular fit assumes an isotropic effective index while the elliptical and
hyperbolic cases are for an anisotropic index of refraction arising from different ε and µ
in different crystallographic directions. Previous models fit the wave vector curve
qualitatively utilizing only an effective index of refraction based on ε as the actual
structure only involves a modulation of the dielectric constant
2839
. A more general
model allowing both ε and µ to affect the index was investigated.
Since only the product εµ is proportional to the index, either property can be fit
for calculating the effective index of refraction. However, when considering the two
dimensional case, the set of ε and µ values which affect each polarization are fixed, thus
for the TE and TM modes, the values of ε and µ used to fit the index profile are restricted.
In the TM mode propagating in the zdirection and xdirection perpendicular to the plane
of the slab, only the H
z
, H
y
, and E
x
components exist, thus only the z component of the
dielectric constant appears, and the shape of the wave vector contour cannot be modified
from a circle without introducing anisotropy in the µ
x
and µ
y
values. For the TE mode,
the opposite applies as an anisotropic dielectric constant is sufficient to modify the shape
of the wave vector curve. Both the TM and TE mode band structure show the same
concavity reversal which gives a significant conclusion that a periodic structure with
modulation only in ε can result in an effective anisotropy in µ. This effect is attributed to
the multiple reflections off of the curved surfaces of the periodic structure which allows a
modulation in the dielectric constant to affect the evolution of the magnetic field. The
models for the ε and µ are as follows:
35
⎥
⎥
⎥
⎦
⎤
⎢
⎢
⎢
⎣
⎡
=
z
y
x
ε
ε
ε
ε
00
00
00
, and
⎥
⎥
⎥
⎦
⎤
⎢
⎢
⎢
⎣
⎡
=
z
y
x
µ
µ
µ
µ
00
00
00
Equation 17
Curve fitting of the wave vector curves were utilized to calculate the following effective
index values:
εµ
=
circle
n
ModeTE
xy
ModeTM
yxphasehyperbolaellipsenpropagatio
k
nn
__
/_
µεµε
ω
====
ModeTE
xz
ModeTM
zxtranshyperbolaellipsetransverse
nn
__
/_
µεµε ===
Equation 18
where n
circle
is positive for convex and negative for concave curvature; n
phase
is the same
for both elliptical and hyperbolic fits; and n
trans
is real for elliptical and imaginary for
hyperbolic fit. Zdirection propagation was assumed for these calculations. Utilizing
these models for the index of refraction, the parabolic wave equation was solved for
propagation of a Gaussian beam. The circular fit model simply replaces the index of
refraction with that calculated from the curvature. The beam size, longitudinal phase, and
radial phase parameters for the Gaussian beam utilizing the circular fit model are:
( )
⎟
⎟
⎠
⎞
⎜
⎜
⎝
⎛
⎟
⎟
⎠
⎞
⎜
⎜
⎝
⎛
+=
2
2
0
0
2
0
2
1
wn
z
wzw
circle
circle
π
λ
( )
z
n
wn
z
z
circle
circle
circleallongitudin
0
2
0
0
1
_
2
2
tan
λ
π
π
λ
+
⎟
⎟
⎠
⎞
⎜
⎜
⎝
⎛
−=Φ
−
36
⎟
⎟
⎠
⎞
⎜
⎜
⎝
⎛
⎟
⎟
⎠
⎞
⎜
⎜
⎝
⎛
+
=Φ
2
0
2
0
2
_
1
λ
π
π
z
wn
z
yn
circle
circle
circleradial
Equation 19
where the w
0
is half of the beam size at the waste; and λ
0
is the wavelength in free space.
For the elliptical and hyperbolic case, the conventional approach to solving this problem
includes a coordinate transformation to restate the problem into an isotropic index in an
anisotropic coordinate system
64,65
, but for the case considered here where only the ΓM
direction is of interest, the problem can be solved without a coordinate transformation
and intuitive results can be obtained. First, all of the ε and µ are normalized to the zaxis
values as propagation in the zdirection is assumed:
⎥
⎥
⎥
⎦
⎤
⎢
⎢
⎢
⎣
⎡
=
⎥
⎥
⎥
⎦
⎤
⎢
⎢
⎢
⎣
⎡
=
100
00
00
00
00
00
/
/
zy
zx
z
z
y
x
ε
ε
ε
ε
ε
ε
ε
⎥
⎥
⎥
⎦
⎤
⎢
⎢
⎢
⎣
⎡
=
⎥
⎥
⎥
⎦
⎤
⎢
⎢
⎢
⎣
⎡
=
100
00
00
00
00
00
/
/
zy
zx
z
z
y
x
µ
µ
µ
µ
µ
µ
µ
Equation 20
Then, the normalized values can be used to obtain a value for the divergences of the
fields, which are not zero anymore due to the anisotropic media:
( )
( )
y
E
x
E
E
y
zy
x
zx
∂
∂
−+
∂
∂
−=•∇
//
11 εε
( )
( )
y
H
x
H
H
y
zy
x
zx
∂
∂
−+
∂
∂
−=•∇
//
11 µµ
Equation 21
37
Substituting these values into the wave equation form of the Maxwell’s Equation and
making the twodimensional approximation in the xdirection, the following two
equations can be obtained for the TE and TM, modes respectively:
0
2
2
2
/
2
2
=
⎟
⎟
⎠
⎞
⎜
⎜
⎝
⎛
+
∂
∂
+
∂
∂
x
x
yz
x
Ek
z
E
y
E
µ
0
2
2
2
/
2
2
=
⎟
⎟
⎠
⎞
⎜
⎜
⎝
⎛
+
∂
∂
+
∂
∂
x
x
yz
x
Hk
z
H
y
H
ε
Equation 22
Only one extra factor, the µ
z/y
and ε
z/y
is necessary to account for the anisotropy in the
material. Solving for the Gaussian beam parameters results in
63
:
( )
⎟
⎟
⎟
⎠
⎞
⎜
⎜
⎜
⎝
⎛
⎟
⎟
⎠
⎞
⎜
⎜
⎝
⎛
+=
2
2
0
0
2
0
2
/
1
wnn
z
wzw
phasefactor
hyperbolaellipse
π
λ
( )
z
n
wnn
z
z
phase
phasefactor
hyperbolaellipseallongitudin
0
2
0
0
1
/_
2
2
tan
λ
π
π
λ
+
⎟
⎟
⎠
⎞
⎜
⎜
⎝
⎛
−=Φ
−
⎟
⎟
⎟
⎠
⎞
⎜
⎜
⎜
⎝
⎛
⎟
⎟
⎠
⎞
⎜
⎜
⎝
⎛
+
=Φ
2
0
2
0
2
/_
1
λ
π
π
z
wnn
z
ynn
phasefactor
phasefactor
hyperbolaellipseradial
where,
ModeTEyzModeTMyz
phase
trans
factor
n
n
n
__/__/
2
εµ ==
⎟
⎟
⎠
⎞
⎜
⎜
⎝
⎛
=
Equation 23
The form of the solution parallels the solution for the isotropic case with the appropriate
index factor placed in the appropriate locations. Even though the solution is rather trivial,
the interpretation provides extensive insight into the propagation properties of the
Gaussian beam in such an anisotropic media.
38
The case for the circular fit is discussed first for reference. Since the index was
increased for this case compared to the n
phase
value which can be determined from the ω
and k values directly, the circular model predicts that the beam can travel an increased
length by a factor of n
circle
/n
phase
while maintaining the same beam spread since
substitution of z by zn
circle
/n
phase
returns the equation back to the case for an isotropic
material where the index of refraction is the same as the phase velocity index of
refraction. The main discrepancy of this model is in the longitudinal component of the
beam, which oscillates at unrealistically short wavelengths as n
circle
Enter the password to open this PDF file:
File name:

File size:

Title:

Author:

Subject:

Keywords:

Creation Date:

Modification Date:

Creator:

PDF Producer:

PDF Version:

Page Count:

Preparing document for printing…
0%
Σχόλια 0
Συνδεθείτε για να κοινοποιήσετε σχόλιο